1 / 21

210 likes | 352 Views

The free carrier transport properties in proton and neutron irradiated Si(Ge) (and comparison with Si). J.Vaitkus, V.Rumbauskas, L.Makarenko 1 , A.Mekys, J.Storasta. Vilnius University, Institute of Applied Research, Vilnius, Lithuania 1 Belorussian university, Minsk, Belorussia.

Download Presentation
## The free carrier transport properties in proton and neutron irradiated Si(Ge)

**An Image/Link below is provided (as is) to download presentation**
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.
Content is provided to you AS IS for your information and personal use only.
Download presentation by click this link.
While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
During download, if you can't get a presentation, the file might be deleted by the publisher.

E N D

**The free carrier transport properties in proton and neutron**irradiated Si(Ge) (and comparison with Si) J.Vaitkus, V.Rumbauskas, L.Makarenko1, A.Mekys, J.Storasta Vilnius University, Institute of Applied Research, Vilnius, Lithuania 1Belorussian university, Minsk, Belorussia J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**The important questions: 1) Are the changes in the**semiconductor homogeneity caused by the irradiation? 2) What kind of inhomogeneities are induced by crystal growth (different doping) and treatments?The answers can be find by investigation of the transport properties of free carriers. J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Basic principle**V - + A Hall and magnetoresistance effects are “simple classical effects” demonstrating the transport properties of free carrier. f =1 in a thin sample J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Complications of the Basic principle in the nonhonogeneous**sample V - + A Scattering by large defects: J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Inhomogeneities**V. G. Karpov, A. J. Shik and B. I. Schklovskij (1982): The cells of typical clusters: I, II and III. Dashed lines indicates the equipotential lines Also, a bit different analyse: W. Siegel, S. Schulte, C. Reichel, G. Kuhnel, J. Monecke. „Anomalous temperature dependence of the Hall mobility in undoped bulk GaAs“. J. Appl. Phys., Vol. 82, No. 8, pp.3832-3835 (1997) J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Single crystals Si (WODEAN1 series)**• The weak dependence on T was observed in low irradiated samples • The Hall and magnetoresistance mobility behavior was different. • Anomalous Hall mobility dependence on T was observed Irradiation by neutrons J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**A new series: Minsk-KEF**Irradiation by electrons (6MeV) to create only the point defects Magnetoresistivity mobility values are typical for good n-type Si. At higher doses of irradiation the Hall signal lowers at low T similarly to the case of clusters. Large scale electric potential disturbance occurs. J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**KDB conductivity (irradiated 4 MeV electrons)**The conductivity in the initial samples decreases with T. This is the case when the carrier density changes less than the mobility. At the higher irradiation doses the conductivity decreases. The greater sample volume is damaged. J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**KDB density**Thermal activation from the density show some clear values. J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**KEF conductivity**Similar situation as in KDB samples. But the conductivity decreases less for the greater doses while it decreases more for lower doses. J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**KEF density**Thermal activation from the density show some clear values. J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Si(Ge)Cz SiGe crystals were grown in Leibniz Institute for**Crystal Growth, Berlin, Germany by N.V. Abrosimov Due to deformation of the lattice the increase of radiation hardness is waited. It exists experience to destroy the dislocation net in GaAs by adding isovalent impurity In. What is happening in transport properties? The start of the analyze cycle. J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Hall mobility in Si(Ge) (neutron irradiation)**Adding of Ge enhances the hole mobility. Irradiation 1e12 cm-2 increases the Hall mobility but the 1e13 cm-2 decreases the Hall mobility in both n-type and p-type (at 200-3000 C) J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Proton irradiated Si(Ge)**J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Proton irradiated Si(Ge)**J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Si(Ge)**Neutron irradiation Proton irradiation J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Neutrons, Si(Ge)**Hall Magnetoresistance J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Conclusions:**• The main peculiarities of transport phenomena are induced by cluster defects. • Hall effect and magnetoresistance measurement allow to reveal these inhomogeneities • The initial studies of low irradiated Si(Ge) were performed. • The irradiation to the higher fluence is the next step. J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**THANK YOU FOR YOUR ATTENTION**J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Hall factor**Hall scattering factor rH is defined by following expressions: The relaxation time for individual scattering process often follows a power law: Variation of Hall scattering factor with total impurity density Nimp. In n-type Si. Experimantal points: -x- 77K, -o- 300K. Solid curves: calculated (from Kirnas et al., 1974) J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012**Inhomogeneities**l1 l1 grain VA R. H. Bube model: l2 VH [R. H. Bube, Appl. Phys. Lett. 13, 136 (1968)] J.Vaitkus, L.Makarenko et all. RD50, CERN, 2012

More Related